Optical properties of silicon nanowire arrays formed by metal-assisted chemical etching: evidences for light localization effect
© Osminkina et al.; licensee Springer. 2012
Received: 30 April 2012
Accepted: 10 August 2012
Published: 25 September 2012
We study the structure and optical properties of arrays of silicon nanowires (SiNWs) with a mean diameter of approximately 100 nm and length of about 1–25 μm formed on crystalline silicon (c-Si) substrates by using metal-assisted chemical etching in hydrofluoric acid solutions. In the middle infrared spectral region, the reflectance and transmittance of the formed SiNW arrays can be described in the framework of an effective medium with the effective refractive index of about 1.3 (porosity, approximately 75%), while a strong light scattering for wavelength of 0.3 ÷ 1 μm results in a decrease of the total reflectance of 1%-5%, which cannot be described in the effective medium approximation. The Raman scattering intensity under excitation at approximately 1 μm increases strongly in the sample with SiNWs in comparison with that in c-Si substrate. This effect is related to an increase of the light-matter interaction time due to the strong scattering of the excitation light in SiNW array. The prepared SiNWs are discussed as a kind of ‘black silicon’, which can be formed in a large scale and can be used for photonic applications as well as in molecular sensing.
KeywordsSilicon nanowires Black silicon Raman scattering Light localization
Currently, silicon nanowires (SiNWs) are of great interest due to their potential applications in various fields suchlike microelectronics, optoelectronics, photonics, photovoltaics, biologic, and chemical sensors [1–9]. In particular, SiNWs exhibit a strong optical absorption and rather low reflectance in the visible spectral range [4, 6] as well as in room temperature photoluminescence (PL) [10, 11]. There are several ways to form SiNWs, and the first method is based on vapor–liquid-solid or bottom-up growth catalyzed by noble metal (mostly gold, Au), as firstly proposed by Wagner and Ellis in 1964 . Some years ago, it was demonstrated that SiNWs can be formed by top-down approaches suchlike a reactive ion etching, electrochemical etching, and metal-assisted chemical etching (MACE) [13–19]. Since both the electronic and optical properties of nanostructures are dependent on the method of their preparation, it is of great importance to control the growth and structure of SiNWs.
In the present paper, we study the morphology, microstructure, and optical properties of SiNWs obtained by MACE (assisted by silver nanoparticles) of crystalline silicon (c-Si) in hydrofluoric acid solution. It is shown that the formed SiNWs are characterized by the optical reflection and transmission, which are strongly modified in comparison with those for c-Si substrate. In addition, SiNWs exhibit efficient Raman scattering, and this effect can be interpreted in terms of the strong Anderson-like localization of the excitation light in the SiNW array.
The structural properties of SiNWs were investigated by using a scanning electron microscope (SEM) of Lira Tescan (Tescan USA, PA, USA) and a transmission electron microscope (TEM) of LEO912 AB Omega (Carl Zeiss SMT AG Oberckochen, Germany). The optical reflectance and transmittance spectra in the region of 500–10,000 cm−1 were studied with a Fourier-transform infrared (FTIR) spectrometer of Bruker IFS 66v/S (Bruker Corporation, Billerica, MA, USA). The spectra were measured at normal incidence. The infrared (IR) PL and Raman spectra under excitation with a CW Nd:YAG laser at 1.064 μm (excitation intensity approximately 100 mW; spot size approximately 2 mm) were measured in a back scattering geometry with the same spectrometer equipped with an FRA-106 unit. The total reflectance spectra in the region from 300 to 2,000 nm were measured with Perkin Elmer Lambda 950 spectrometer (PerkinElmer Inc., Waltham, MA, USA) equipped with an integrating sphere. All measurements were carried out at room temperature in air.
Results and discussion
Figure 1b shows a TEM image of individual SiNW. The diameter, D, of SiNW is about 100 nm and D is nearly constant through the whole SiNW length, which was varied from 2 to 60 μm in the prepared samples. The outer surface of SINW is rough in nanoscale  and the nanostructure surface layer, d, is visible as less dark regions in the TEM image of SiNW sides.
Figure 1b,c shows typical large-scale cross-sectional SEM images of a sample with SiNWs. One can see that SiNWs look like quasi-ordered arrays with preferential orientation along the  crystallographic direction. The length of SiNWs, L, was nearly proportional to the etching time in agreement with results of .
Since the growth of SiNWs is controlled by the redox process initiated by silver (Ag) nanoparticles, they are observed at the interface SiNWs/c-Si for as-prepared samples (Figure 1c). The Ag nanoparticles could be easily removed from the interface by etching the samples in concentrated HNO3 (see Figure 1d). It is important to note that the etching in HNO3 did not lead to remarkable changes of the structure properties of SiNWs monitored by means of TEM and SEM.
The reflection coefficient (Figure 2a) and transmittance (Figure 2b) of SiNWs are rather high in the spectral region of wave numbers below 5,000 cm−1 (λ > 2 μm). Since in this spectral region D < < λ the SiNW array can be considered as an effective optical medium with the effective refractive index neff. The latter can be estimated from the interference oscillations in the first derivative of the reflection coefficient (see inset in Figure 2a) and it is accounted to be 1.3 ± 0.1 in the spectral range of 2,000-6,000 cm−1. According to the effective medium approximation (Bruggeman model, see for example review ), the value of neff=1.3 corresponds to the porosity of SiNW array to be about P = 75%. This value seems to be formed by both the spatial density of SiNW array and the local porosity of SiNW sides. Note that the reflectance is higher and the transmittance is lower for the samples with Ag nanoparticles (blue curves in Figure 2). This effect is obviously explained by the contribution of the metal fraction to the effective dielectric function. Both the reflection coefficient (Figure 2a) and the transmittance (Figure 2b) of SiNWs decrease in the high frequency range (λ < 2 μm) due to the light scattering.
The Raman scattering intensity increases strongly for the samples with SiNWs in comparison with the corresponding value of c-Si substrate (see inset in Figure 4a). The enhancement of the Raman scattering is several times larger for the samples without Ag nanoparticles. This fact can be explained by taking into account the additional optical losses induced by Ag nanoparticles, while the well-known effect of the local field enhancement near metallic particles seems to be negligible in the investigated structures.
Figure 4b shows that the Raman scattering intensity of SiNWs is not proportional to the length of SiNW. The corresponding dependence is well approximated by a logarithmic function as it is shown in the inset of Figure 4b. This logarithmic dependence indicates a diffusive origin of propagation of the excitation radiation and/or detected light. It is worth to notice that the Raman scattering from the samples with SiNWs was completely depolarized, while the signal of the substrate demonstrated the characteristic polarization dependence, which was inherent for the (100)-oriented c-Si wafer .
Where ISiNW and Ibulk are the measured Raman intensities for the samples with SiNWs and for the c-Si substrate, respectively; VSiNW and Vbulk are the corresponding SiNWs and the c-Si substrate volumes probed by the excitation light. Because the Stokes component of the Raman scattering in c-Si excited at 1.06 μm is weak-absorbed (absorption coefficient at approximately 2 cm−1), the value of Vbulk is about the thickness of c-Si substrate, which was equal to L0 = 400 μm, multiplied by the excitation spot area (S ≈ 4 mm2). The excited volume of SiNWs is approximately proportional to the length of SiNWs corrected to the porosity, i.e., .
According to Equation 1, RE is approximately 103 for the sample of SiNWs with L = 2 μm. The value of RE decreases for the samples with larger L. This fact indicates that the main contribution to the Raman scattering enhancement is induced on the thin (L < 2 μm) top layer of the SiNW arrays.
The enhancement of the Raman scattering in SiNWs can be interpreted as increasing the excitation intensity of SiNWs because of the partial light localization in inhomogeneous optical medium . Such kind of light localization was observed in different porous semiconductors as GaP, TiO2, and Si (see for example a review in  and references therein); and it is analogous for the Anderson localization for electrons in amorphous semiconductors .
Another explanation of the enhanced Raman scattering in SiNW array is based on consideration of a resonant enhancement of the incident electromagnetic radiation by individual SiNWs as demonstrated in . While both explanations are possible, the concept of light localization allows us to understand better the observed dependence of the Raman scattering intensity on L (see Figure 4b).
where is the interaction time of photon with the c-Si substrate (c is the velocity of light in vacuum; nbulk is the refractive index of c-Si). Since for the employed substrate s we can estimate the lower limit of τSiNW at approximately 10-8 s.
The strong shortening of light-matter interaction time in SiNW array is obviously interesting for various photonic applications as nonlinear optical conversion of the light frequency and for the duration of short laser pulses . Furthermore, the extremely low total reflectance of SiNW array in the ultraviolet (UV)-visible and near IR spectral ranges can be used to increase the absorbance of solar cells and other photovoltaic devices. Indeed, the application of SiNWs for new type of solar cell was already demonstrated .
Another field of application of the observed effect of light localization is the sensing of molecules incorporated or/and absorbed in SiNW array. The detection of enhanced molecular response at characteristic vibration frequencies can be realized by means of the IR reflectance/transmittance and Raman spectroscopy. The possibility of the latter was recently demonstrated for grooved Si structure with partial light localization .
The obtained experimental data on the structure and optical properties of silicon nanowire arrays prepared by metal-assisted chemical etching of c-Si in hydrofluoric acid solutions demonstrate new possibilities for tailoring the physical properties of Si-based nanostructures. The reflectance and transmittance of SiNWs depend on the presence of Ag nanoparticles, which result in the optical losses in the samples. In the middle IR spectral range, the formed arrays of SiNWs act as the effective medium with the low refractive index, which can be used as anti-reflective coating for photonic devices. The formed SiNW arrays demonstrate a strong decrease of the total reflectance near 1%-4% in the spectral region of 300 ÷ 1,000 nm and they can be used as a kind of ‘black silicon’, which can be formed by the simple chemical method in a large scale. The observed low reflectance correlates with the strong increase of the Raman scattering efficiency in SiNWs in comparison with that for c-Si substrate. The enhancement of the Raman scattering efficiency is interpreted as an evidence of the light localization because of the multiple scattering in SiNW array. The light localization effect in SiNWs can be used in various photonic applications as well as in molecular sensorics.
The work was partially performed at the user facilities center at Lomonosov Moscow State University and supported by the Russian Foundation for Basic Research (projects numbers 11-02-90506 and 11-02-01087) and the Ministry of Education and Science of the Russian Federation (contract numbers 8737 and 16.513.12.3010). VAS gratefully acknowledges the financial support by the European Commission in part of the European Project in the framework of FP7, ‘ROD-SOL’ (FP7-NMP-227497) and European Regional Development Fund (EFRE-SIFas).
- Yang P, Yan R, Fardy M: Semiconductor nanowire: what’s next? Nano Lett 2010, 10: 1529–1536. 10.1021/nl100665rView Article
- Hu J, Ouyang M, Yang P, Lieber CM: Controlled growth and electrical properties of heterojunctions of carbon nanotubes and silicon nanowires. Nature 1999, 399: 48–51. 10.1038/19941View Article
- Föll H, Hartz H, Ossei-Wusu E, Carstensen J, Riemenschneider O: Si nanowire arrays as anodes in Li ion batteries. Phys Status Solidi RRL 2010, 4(1,2):4–6.View Article
- Bronstrup G, Jahr N, Leiterer C, Csaki A, Fritzsche W, Christiansen S: Optical properties of individual silicon nanowires for photonic devices. ACS Nano 2010, 4(12):7113–7122. 10.1021/nn101076tView Article
- Kelzenberg MD, Turner-Evans DB, Kayes BM, Filler MA, Putnam MC, Lewis NS, Atwater HA: Photovoltaic measurements in single-nanowire silicon solar cells. Nano Lett 2008, 8: 710–714. 10.1021/nl072622pView Article
- Sivakov V, Andrä G, Gawlik A, Berger A, Plentz J, Falk F, Christiansen SH: Silicon nanowire-based solar cells on glass: synthesis, optical properties, and cell parameters. Nano Lett 2009, 9: 1549–1554. 10.1021/nl803641fView Article
- Hochbaum AI, Fan R, He R, Yang P: Controlled growth of Si nanowire arrays for device integration. Nano Lett 2005, 5: 457–460. 10.1021/nl047990xView Article
- Cui Y, Wei Q, Park H, Lieber CM: Nanowire nanosensors for highly sensitive and selective detection of biological and chemical species. Science 2001, 293: 1289–1292. 10.1126/science.1062711View Article
- Wang X, Ozkan CS: Multisegment nanowire sensors for the detection of DNA molecules. Nano Lett 2008, 8(2):398–404. 10.1021/nl071180eView Article
- Sivakov VA, Voigt F, Berger A, Bauer G, Christiansen SH: Roughness of silicon nanowire sidewalls and room temperature photoluminescence. Phys Rev B 2010, 82: 125446–125452.View Article
- Timoshenko VY, Gonchar KA, Golovan LA, Efimova AI, Sivakov VA, Dellith A, Christiansen SH: Photoluminescence and Raman scattering in arrays of silicon nanowires. J Nanoelectr Optoelectr 2011, 6(4):519–524. 10.1166/jno.2011.1205View Article
- Wagner RS, Ellis WC: Vapor–liquid-solid mechanism of single crystal growth. Appl Phys Lett 1964, 4: 89–90. 10.1063/1.1753975View Article
- Huang Z, Fang H, Zhu J: Fabrication of silicon nanowire arrays with controlled diameter, length, and density. Adv Mater 2007, 19: 744–748. 10.1002/adma.200600892View Article
- Cui Y, Lauhon LJ, Gudiksen MS, Wang J, Lieber CM: Diameter-controlled synthesis of single-crystal silicon nanowires. Appl Phys Lett 2001, 78: 2214–2216. 10.1063/1.1363692View Article
- Ross FM, Tersoff J, Reuter MC: Sawtooth faceting in silicon nanowires. Phys Rev Lett 2005, 95: 146104–146108.View Article
- Boarino L, Imbraguglio D, Enrico E, De Leo N, Celegato F, Tiberto P, Pugno N, Amato G: Fabrication of ordered silicon nanopillars and nanowires by self-assembly and metal-assisted etching. Phys Status Solidi A 2011, 208(6):1412–1416. 10.1002/pssa.201000182View Article
- Huang Z, Geyer N, Werner P, de Boor J, Gösele U: Metal-assisted chemical etching of silicon: a review. Adv Mater 2011, 23: 285–308. 10.1002/adma.201001784View Article
- Nassiopoulou AG, Gianneta V, Katsogridakis C: Si nanowires by a single-step metal-assisted chemical etching process on lithographically defined areas: formation kinetics. Nano Res Let 2011, 6: 597. 10.1186/1556-276X-6-597View Article
- Sivakov VA, Brönstrup G, Pecz B, Berger A, Radnoczi GZ, Krause M, Christiansen SH: Realization of vertical and zigzag single crystalline silicon nanowire architectures. J Phys Chem C 2010, 114: 3798–3803. 10.1021/jp909946xView Article
- Golovan LA, Timoshenko VY, Kashkarov PK: Optical properties of porous-system-based nanocomposites. Phys Usp 2007, 50(6):595–612. 10.1070/PU2007v050n06ABEH006257View Article
- Sze SM: Physics of Semiconductor Devices. New York: Wiley; 1981.
- Kovalev D, Heckler H, Polisski G, Koch F: Optical properties of Si nanocrystals. Phys Stat Sol (b) 1999, 215: 871–932. 10.1002/(SICI)1521-3951(199910)215:2<871::AID-PSSB871>3.0.CO;2-9View Article
- Cao L, Nabet B, Spanier JE: Enhanced Raman scattering from individual semiconductor nanocones and nanowires. Phys Rev Lett 2006, 96: 157402.View Article
- Madan A, Shaw MP: The Physics and Application of Amorphous Semiconductors. Boston: Academic Press; 1988.
- Gonchar KA, Golovan LA, Timoshenko VY, Sivakov VA, Christiansen S: Effects of light localization in photoluminescence and Raman scattering in silicon nanostructures. Bull Russ Acad Sci Phys 2010, 74(12):1712–1714. 10.3103/S1062873810120208View Article
- Mamichev DA, Timoshenko VY, Zoteyev AV, Golovan LA, Krutkova EY, Laktyunkin AV, Kashkarov PK, Astrova EV, Perova TS: Enhanced Raman scattering in grooved silicon matrix. Phys Stat Sol B 2009, 246: 173–176. 10.1002/pssb.200844163View Article
This article is published under license to BioMed Central Ltd. This is an Open Access article distributed under the terms of the Creative Commons Attribution License (http://creativecommons.org/licenses/by/2.0), which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly cited.